Hall-conductivity sign change and fluctuations in amorphous Nbx
Nobuhito Kokubo, Jan Aarts, and Peter H. Kes
Kamerlingh Onnes Laboratory, Leiden University, P. O. Box 9504, 2300 RA Leiden, The Netherlands
共Received 8 December 2000; published 11 June 2001兲
The sign change in the Hall conductivity has been studied in thin amorphous Nb1⫺xGex(x⬇0.3) films. By changing the film thickness it is shown that the field at which the sign reversal occurs shifts to lower values 共from above to below the mean-field transition field Hc2) with increasing film thickness. This effect can be understood in terms of a competition between a positive-normal and a negative-fluctuation contribution to the Hall conductivity.
DOI: 10.1103/PhysRevB.64.014507 PACS number共s兲: 74.25.Fy, 74.40.⫹k, 74.80.Bj
One of the puzzling and intriguing phenomena in type-II superconductors is the sign change in the Hall effect near the mean-field transition at the upper critical field Hc2. Such a
Hall anomaly has been observed in some conventional
low-Tc superconductors, such as, moderately disordered Nb and
V共Ref. 1兲and amorphous MoSi共Refs. 2 and 3兲and MoGe
共Ref. 4兲 films, as well as most high-Tc superconductors 共HTSC兲.5 Hagen et al.5 pointed out the importance of the electron mean-free path for the Hall anomaly and concluded that very clean and very dirty materials do not show Hall anomalies. However, studies on amorphous dirty supercon-ductors contradict this conclusion.2–4
Recent phenomenological approaches based on the time-dependent Ginzburg-Landau共TDGL兲equation have qualita-tively explained the sign anomaly.6–8 In these theories, the sign reversal is just a consequence of the difference in sign between the normal共or quasiparticle兲term and the supercon-ducting fluctuation共or vortex flow兲term of the Hall conduc-tivity. Several authors9–12 have derived the sign of the fluc-tuation共vortex flow兲term from the TDGL equation for BCS superconductors. Recent experimental studies13 on HTSC’s have pointed out that the sign predictions of these theories are not correct for HTSC’s, but they should be valid for BCS superconductors.
Even if the sign of the Hall-fluctuation conductivity were clear, its temperature and field dependence is a matter of discussion. Recent experimental studies on YBa2Cu3O7⫺␦ films14–16 and single-crystalline Bi2Sr2CaCu2O8⫹␦ and Bi1.95Sr1.65La0.4CuO6⫹␦共Ref. 17兲have observed that the sign change takes place above Hc2, while other studies have
claimed that the sign anomaly takes place below Hc2. In this
problem, the definition of Hc2as well as the temperature and
field dependence of the Hall-fluctuation conductivity is very important.
As reported in conventional amorphous films18 as well as HTSC’s, the longitudinal conductivity in a perpendicular magnetic field shows a smooth crossover from the paracon-ducting regime to flux-flow regime around Hc2, which is
strikingly different from the picture of the conventional fluc-tuation theory in which the conductivity due to the direct fluctuation contributions of the Aslamazov-Larkin共AL兲 pro-cess diverges at Hc2.
Thus, it was difficult to define Hc2
correctly from the fluctuation theory. Recent TDGL
theories,6 however, have successfully explained the smooth crossover around Hc2by taking into account the interaction term of superconducting fluctuations of the AL process within the Hartree approximation. Later, Ullah and Dorsey
共UD兲 共Ref. 7兲developed this further and proposed a scaling theory for the longitudinal and Hall conductivities. This scal-ing approach is very useful to determine Hc2correctly and to
describe the field and temperature dependence of the conduc-tivities.
In this paper, we present measurements and analysis of the longitudinal and Hall resistivities xx and y x for thin
amorphous 共a-兲 Nb1⫺xGex (x⬇0.3) films (Tc⬇3 K) ac-cording to the TDGL theories. We confirm that the smooth crossover in the longitudinal conductivity around Hc2is well
explained by the UD scaling theory as was found previously,20 and determine Hc2. We then show that for the
thinner films the sign change in the Hall conductivity takes place above Hc2. Contrary to results on HTSC’s, we show that the sign of the Hall conductivity is consistent with the TDGL theory for BCS superconductors. We discuss the ori-gin of the sign reversal observed here.
The films used in this study were deposited by rf sputter-ing on Si substrates held at room temperature in a system with a base pressure of 10⫺6 mbar, using 10⫺2 mbar Ar gas as a sputtering gas. The thicknesses used were 16, 34, 60, and 163 nm. X-ray diffraction showed the films to be amor-phous. The average composition for each film was deter-mined by electron-microprobe analysis. The distribution in the composition ␦x is less than 1%. The superconducting
mean-field transition temperature in zero field, Tc, was
de-termined from the temperature dependence of resistivity by using the AL fluctuation theory.21 From a previous system-atic study on a-Nb1⫺xGexfilms,22the distribution of Tcdue to ␦x is estimated to be less than 18 mK (␦T/Tcⱗ6
⫻10⫺3) around x⫽0.3. Except for the film thickness, these films have the following identical parameters; the average composition x⬇0.3, Tc⬇3 K, the normal-state resistivity
n ⬇2.2 ⍀m, S⬅⫺d(
0Hc2)/dT兩Tc⬇2 T/K, the
eight voltage and two current contacts. The longitudinal and Hall resistivities are measured by a conventional dc four-probe method. The longitudinal component due to the mis-alignment in the Hall probes was subtracted by reversing the field direction. The films are immersed in liquid 4He to ob-tain good thermal contact. The magnetic field is normal to the film surface. The normal resistivity xxn in the tempera-ture range of 1.5 K⬍T⬍5 K has a small temperature coef-ficient (xxn )⫺1dnxx/dT⬃⫺10⫺4 K⫺1.
III. RESULT AND DISCUSSION
In this study,xx(⫽Ex/Jx) andy x(⫽Ey/Jx) were
mea-sured as a function of H (兩0H兩⬉8 T) at various T. Figures 1共a兲 and 1共b兲show the field dependence of the longitudinal xx关⬅xx/(xx
2 )兴 and Hall conductivities
xy 关⬅y x/(xx
2 )兴 at different T for the 34-nm-thick film
with Tc⫽2.77 K. To reduce the effect of pinning in the
mixed state, the measuring current density J was selected to be 1.4⫻107 A/m2 that is much higher than the depinning current density Jc(⬃105 A/m2), but smaller than the
depair-ing current density (⬃1010 A/m2).
Far above Tc, xx is field independent whilexy is
di-rectly proportional to H, that is, the normal-state Hall effect appears. The normal-state Hall conductivity xy
has a posi-tive sign. Within the Drude model, the normal-state Hall angle, tanHn , is given by
tanHn⬅xyn /xxn ⫽c, 共1兲
where c is the cyclotron frequency and is the elastic scattering time of electrons. Compared with typical result on HTSC’s (c⬃10⫺2 at0H⫽1 T), the present films have very small value ofc⬃10⫺5at0H⫽1 T, indicating the very small mean-free path to be expected for amorphous metals.
Near and below Tc one can clearly see that xy changes sign at a certain field H*in Fig. 1共b兲. We do not observe any second sign change below H*, in contrast to what has been reported for several HTSC’s.23Far above H*, xy recovers
the direct proportionality to H and the normal-state Hall ef-fect appears again, indicating that the superconducting fluc-tuations are completely suppressed by magnetic field. We therefore can define xy
below Tc unambiguously.
In order to determine Hc2, we use the UD scaling theory.
According to this theory, the longitudinal conductivity is composed of the normal 共or quasiparticle兲 term xxn and superconducting-fluctuation共or vortex-flow兲term␦xx, and
xx⫽xx n ⫹␦
␦xx interpolates smoothly from the paraconducting regime
to flux-flow regime around Hc2and obeys universal scaling functions F˜⫾ where F˜⫹(F˜⫺) is the scaling function for H ⬎Hc2(H⬍Hc2). These functions depend on the
dimension-ality governed by the ratio of the film thickness d and the length scale for fluctuations of the order parameter near
Hc2. For the thickness of the films in this study we can apply
two-dimensional 共2D兲 scaling functions.20 At each T we identify xxn withxx taken at a field 共typically 7 T兲where
xy depends linearly on field and xx is field independent.
␦xx is obtained by subtracting xx
xx. Figure 2
shows a typical scaling result. Here, the data are plotted above Hc2(T)/3 where the lowest Landau level 共LLL兲
ap-proximation for the scaling functions is valid.20 One can clearly see that the scaled longitudinal fluctuation conductiv-ity F˜xx2D兵⬅␦xx/关Cxx
(A02Dt/h)1/2兴其 collapses on two uni-versal curves F˜⫾ as a function of the scaled field x2Dgiven by x2D⬅⑀H/
th, with ⑀H⫽0关H⫺Hc2(T)兴/STc,
al-though deviations are visible at large 兩x2D兩. Here, t⫽T/Tc
and h⫽0H/STc are normalized temperature and field,
re-spectively. C is related to the real part of the relaxation time of the order parameter ␥⫽␥1⫹i␥2. We take a dirty limit value of C⫽1.447.20The strength of thermal fluctuations for 2D system, A02D, is given by A02D⫽4
FIG. 1. The field dependence of 共a兲 the longitudinal,共b兲 Hall, and共c兲Hall-fluctuation conductivities at different T of 2.08 K (䊊), 2.20 K (䊐), 2.47 K (䉭), 2.60 K (〫), and 3.71 K (ⵜ) for a 34-nm-thick film. The short and long arrows denote the sign-reversal field H* and the mean-field transition field Hc2,
Gi(⬇5⫻10⫺6) is the Ginzburg number.24 Very close to Hc2, deviations due to the inhomogeneity in the composition
␦x become apparent. Hence, we do not plot the data in fields 兩⑀H兩⬍(1/2)␦Tc/Tc⬇3⫻10⫺3, which roughly corresponds
to 兩x2D兩⬍0.2. In such a scaling plot, the unknown param-eters are S and Hc2(T). In the temperature range close to Tc,
they are connected by the simple relation Hc2(T)⫽S(Tc
⫺T). We first determine S from the scaling collapse of the
data close to Tcand this S value is used to determine Hc2far
below Tc in the scaling analysis. Thus, we can unambigu-ously determine Hc2from the scaling collapse of the data.
Before proceeding to the result of the Hc2 line, we com-pare the scaling functions F˜⫾with those predicted in the UD theory. The UD theory implies that the 2D universal func-tions F˜⫾2Din the high-field limit are given by
if the pinning effect in the flux-flow regime is negligible and the fluctuation conductivity in the paraconducting regime is dominated by the direct fluctuation contributions of the AL process. These functions are applicable to the field range where the LLL is satisfied. The solid lines in Fig. 2共a兲denote these universal functions. F˜⫾ agrees well with F˜⫾2D near
Hc2(⫺1ⱗx2Dⱗ6), while deviations are visible in the large
兩x2D兩 regime. In the paraconducting regime, F˜⫹ decreases much faster than F˜⫹2D above x2D⬇6. Such a rapid decrease in␦xxwas also observed far above Hc2in amorphous thick
films and attributed qualitatively to a phenomenological short-wavelength cutoff in the fluctuation spectrum.25For the other films (d⫽16 and 60 nm兲 except for the thickest film (d⫽163 nm),26similar deviation of F˜⫹begins to appear at
almost the same value of x2D⬇6, although the physical ori-gin of the short-wavelength cutoff is not clear. The definition of xxn does not affect this behavior because the field at whichxxn is defined is much larger than the fields of interest. Hereafter, we regard x2D⫽6 as the phenomenological boundary below which ␦xx is well described by the UD scaling theory, and discuss our data below this boundary.
From the scaling collapse of ␦xx we obtained the Hc2
line for films with different thicknesses. To compare those results, we plot the normalized mean-field value of 0Hc2/STc(⬅hc2) against normalized temperature T/Tcfor
different films in Fig. 3. Good agreement is seen for Hc2of all films. The solid line represents the mean-field line for the dirty limit in the Werthamer-Helfand-Hohenberg 共WHH兲 theory, which is given by
where⌿ is the digamma function.27The Hc2line obtained is
well approximated by this relation, giving experimental sup-port for the validity of the UD scaling theory.
Next, we turn to results of the Hall-fluctuation conductiv-ity. In the TDGL theories,7 the Hall conductivity also con-sists of a normal共or quasiparticle兲term and a superconduct-ing fluctuation 共or vortex flow兲term,
xy共H,T兲⫽xy n 共
Hence, we subtract xy n
(H,T) from xy(H,T), and plot
␦xy(H,T) against H in Fig. 1共c兲. The plot shows that␦xy
always has a negative sign. Hc2 is denoted by the long
ar-rows. With decreasing H the magnitude of ␦xy increases monotonically and grows as 1/H at low H (ⰆHc2) 共not
shown兲as the TDGL theories predict.28Thus, the sign rever-sal ofxy at H* always takes place when␦xy andxyn are different in sign. Beforehand it is not clear whether or not FIG. 2. The scaled fluctuation conductivity plotted as a function
of兩x2D兩 at different T of 2.08 K, 2.20 K, 2.47 K, and 2.60 K. The
current density J is 2.94⫻107 A/m2except for the curve at 2.08 K where J⫽1.47⫻107 A/m2. The symbols correspond to those in
Fig. 1. The solid curves represent the 2D universal scaling functions F
. S is found to be 2.16 from the scaling collapse of the data taken at 2.47 K and 2.60 K close to Tc⫽2.77 K. The Hc2values
for 2.08 K and 2.20 K are determined from the scaling collapse of the data using this S value.
FIG. 3. 0Hc2/STc plotted as a function of T/Tc for different
films of 16 nm (䊏), 34 nm (䊉), 60 nm (䉱), and 163 nm (⽧) thickness. The solid curve represents the mean-field line in the dirty limit for the WHH theory. The corresponding open symbols show
0H*/STcfor the same films plotted against T/Tc. The dashed and
dashed-dotted lines represent the phenomenological boundaries
H* is above Hc2, becausexy n
and␦xy depend in different
ways on the electronic structure of the material. As one can see in Fig. 3, in the thinnest film H* 共denoted by open sym-bols兲 is always above Hc2 but below the phenomenological boundary where scaling analysis starts to fail. It may be worth pointing out that H* decreases monotonically with rising T and terminates finally at a certain T* above Tc0 in
zero field. With increasing d, H* moves systematically closer to Hc2 and it finally shifts below 共but very close to兲
Hc2 for the thickest film, implying that the contribution of
the negative ␦xy to positivexy n
decreases with increasing
d. These results support the view that enhancing the
super-conducting fluctuations by reducing d leads to an increasing negative Hall conductivity working against positive xyn , which is responsible for the sign reversal above Hc2.
We now discuss the field and temperature dependences of ␦xy, in comparison with the UD scaling theory. According
to this theory,␦xx and␦xy have the same field and
tem-perature dependence and their ratio should be independent of
H and T. Note that ␦xy/␦xx⫽⫺␥2/␥1, the ratio of the imaginary and real part of ␥.7 We did not find scaling of ␦xy. A recent study on YBa2Cu3O7⫺␦ films14 has pointed out that the failure of the scaling of␦xycan be attributed to the additional contributions of the Maki-Thompson 共MT兲 process, which are not taken into account in the UD theory. However, the MT process cannot explain the present result because the strong pair-breaking effect in the amorphous dirty films should lead to a small contribution.25,29 As one
can see in the inset of Fig. 4共a兲, contrary to the UD scaling theory, ⫺␦xy/␦xx at Hc2 increases monotonically with
cooling. Similar temperature dependence of ⫺␦xy/␦xx
has been reported for amorphous MoSi films.3We conclude that the main reason for the scaling failure is the temperature dependence of ␥2/␥1. Further microscopic calculations based on the BCS theory are required to explain this effect. The field dependence of ⫺␦xy/␦xx is shown in Fig.
4共a兲for two current densities. In the field range (⫺1ⱗx2D
ⱗ6) where ␦xx follows the UD scaling theory, ⫺␦xy/␦xx is independent of J and depends only weakly
on x2D. As one can see in Fig. 4共b兲, however, in the same field range both conductivities change almost one decade in magnitude and their dependences on x2D look very similar. Hence, we believe that both␦xx and␦xy in the
paracon-ducting regime (0⭐x2Dⱗ6) are dominated by the direct fluctuation contributions of the AL process and thus the con-tributions of the AL process are responsible for the sign change of the Hall conductivity above Hc2.
Finally, we discuss the origin of the sign inxy n
for our amorphous films. The sign of xyn depends on the sign of the group velocity v关⬅(1/ប)/k兴 of electrons at the Fermi level where is the energy and k is the wave number. Because of the absence of band structure, the amor-phous materials are generally more free-electron-like than their crystalline counterparts. Therefore, the simple amor-phous metals generally have negativexyn because of a posi-tive group velocity (v⬀k⬎0).30 Most of the amorphous transition metals 共TM’s兲, however, have positivexyn .31The origin of this positive xyn has been attributed to the s-d hybridization interaction in the TM, which leads to a nega-tive group velocity (/k⬍0) at the Fermi level if the Fermi energy F lies within the d band.31–33 The
TM-metalloid-type amorphous superconductors NbGe as well as MoGe and MoSi belong to amorphous TM’s and have posi-tive xy
In the TDGL theory based on BCS superconductors by Nishio and Ebisawa,10the sign of␦xy is determined by the
electron-hole asymmetry, i.e., by the sign of ⫺N
F兴 is the energy derivative of the den-sity of states 共DOS兲 N() at the Fermi energy. Numerical calculations of the DOS for, e.g., amorphous Ni imply32that the total DOS near F is dominated by the DOS for the d band whose energy dependence is characterized by a peak near the center of d-bandd and roughly approximated by a
parabolic energy dependence with negative curvature, i.e.,
N()⬀⫺(⫺d)2. Similar energy dependences of the total
DOS have been commonly observed for various amorphous TM-metalloid alloys by photoemission experiments.34 Be-cause Nb is a less than half-filled 4d-band metal, F lies
below the center of the 4d-band 4d. Thus, a-NbGe films have positive N
⬘. The same argument holds for a-MoGe and MoSi, since Mo is also a less than half-filled 4d-band metal. Thus, sgn(␦xy)⫽sgn(⫺N
⬘)⬍0 in both a-NbGe, a-MoGe, and a-MoSi films.2–4These findings give experimental sup-port for the prediction of the sign of ␦xy in the TDGL theory for BCS superconductors.
FIG. 4. 共a兲 The ratio of the fluctuation conductivities,
⫺␦xy/␦xx, plotted as a function of x2D at T⫽2.08 K for the
34-nm-thick film with different J of 1.4 kA/cm2 (䊊) and
4.4 kA/cm2 (䊐).共b兲The corresponding longitudinal (䊊,䊐) and Hall fluctuation conductivities (䊉,䊏) are also plotted as a function of x2D with different J. Inset in共a兲shows the T/Tcdependence of ␥2/␥1(⫽⫺␦xy/␦xx) at Hc2with different thickness of 16 nm
In summary, we have measured the longitudinal and Hall resistivities for thin films of the dirty superconductor
a-Nb1⫺xGex(x⬇0.3) near Hc2. We confirm that␦xxobeys
the 2D scaling functions of the UD fluctuation theory. We find a good agreement of the obtained Hc2 line with the
WHH theory, supporting the scaling procedure. The failure of the scaling collapse of␦xy is attributed to the
tempera-ture dependence of␥2/␥1. The Hall conductivityxyin
thin-ner films shows a sign change at a certain H*that is above
Hc2 but in the regime where xx follows the UD theory.
With increasing film thickness, H*moves closer to Hc2and it finally shifts below共but close to兲Hc2for the thickest film.
The negative contribution of the superconducting fluctua-tions of the AL process working against positive xyn is
re-sponsible for the sign change above Hc2. The negative sign
of ␦xy in the present films is consistent with the
electron-hole asymmetry in the framework of the TDGL theory for BCS superconductors.
We are very grateful to R. Ikeda for useful comments and sending us his manuscripts. We would like to thank Y. Mat-suda for giving us a copy of his unpublished work. We ac-knowledge the experimental assistance of R. Besseling, M.B.S. Hesselberth, G.L.E. van Vliet, R.W.A. Hendrikx, and T.J. Gortenmulder. This work was part of the research pro-gram of the ‘‘Stichting voor Fundamenteel Onderzoek der Materie’’ 共FOM兲, which is financially supported by NWO. One of the authors共N.K.兲was financially supported by JSPS.
1K. Noto, S. Shinzawa, and Y. Muto, Solid State Commun. 18,
2A.W. Smith, T.W. Clinton, C.C. Tsuei, and C.J. Lobb, Phys. Rev.
B 49, 12 927共1994兲.
3A.W. Smith, T.W. Clinton, W. Liu, C.C. Tsuei, A. Pique, Q. Li,
and C.J. Lobb, Phys. Rev. B 56, 2944共1997兲.
4J.M. Graybeal, J. Luo, and W.R. White, Phys. Rev. B 49, 12 923 共1994兲.
5S.J. Hagen, A.W. Smith, M. Rajeswari, J.L. Peng, Z.Y. Li, R.L.
Greene, S.N. Mao, X.X. Xi, S. Bhattacharya, Qi Li, C.J. Lobb, Phys. Rev. B 47, 1064共1993兲.
6R. Ikeda, T. Ohmi, and T. Tsuneto, J. Phys. Soc. Jpn. 58, 1377 共1989兲; 59, 1397共1990兲; 60, 1051共1991兲.
7S. Ullah and A.T. Dorsey, Phys. Rev. B 44, 262共1991兲. 8
N.V. Kopnin and A.V. Lopatin, Phys. Rev. B 51, 15 291共1995兲. 9H. Fukuyama, H. Ebisawa, and T. Tsuzuki, Prog. Theor. Phys.
10T. Nishio and H. Ebisawa, Physica C 290, 43共1997兲.
11A.G. Arnov and A.B. Rapoport, Mod. Phys. Lett. B 6, 1083 共1992兲; A.G. Arnov, S. Hikami, and A.L. Larkin, Phys. Rev. B 51, 3880共1995兲.
12A. van Otterlo, M. Feigel’man, V. Geshkenbein, and G. Blatter,
Phys. Rev. Lett. 75, 3736共1995兲; M.V. Feigel’man, V.B. Gesh-kenbein, A.I. Larkin, and V.M. Vinokur, Pis’ma Zh. E´ ksp. Teor. Fiz. 62, 811共1995兲 关JETP Lett. 62, 834共1995兲兴; D.I. Khomskii and A. Freimuth, Phys. Rev. Lett. 75, 1384共1995兲.
13T. Nagaoka, Y. Matsuda, H. Obara, A. Sawa, T. Terashima, I.
Chong, M. Takano, and M. Suzuki, Phys. Rev. Lett. 80, 3594 共1998兲.
14W. Liu, T.W. Clinton, A.W. Smith, and C.J. Lobb, Phys. Rev. B
55, 11 802共1997兲.
15A.V. Samoilov, Phys. Rev. B 49, 1246共1994兲.
16W. Lang, G. Heine, P. Schwab, X. Z. Wang, and D. Ba¨uerle,
Phys. Rev. B 49, 4209共1994兲.
17R. Jin and H.R. Ott, Phys. Rev. B 53, 9406共1996兲. 18P. Berghuis and P.H. Kes, Phys. Rev. B 47, 262共1992兲. 19For example, K. Maki, J. Low Temp. Phys. 1, 513共1969兲. 20M.H. Theunissen and P.H. Kes, Phys. Rev. B 55, 15 183共1997兲.
21L.G. Aslamazov and A.I. Larkin, Phys. Lett. 26A, 238共1968兲. 22
R. Wo¨rdenweber, A. Pruymboom, and P.H. Kes, J. Low Temp. Phys. 70, 253共1987兲.
23For example, W.N. Kang, B.W. Kang, Q.Y. Chen, J.Z. Wu, S.H.
Yun, A. Gapud, J.Z. Qu, W.K. Chu, D.K. Christen, R. Kerchner, and S.W. Chu, Phys. Rev. B 59, 9031共1999兲.
24C.J. Lobb, Phys. Rev. B 36, 3930共1987兲.
25W.L. Johnson, C.C. Tsuei, and P. Chaudhari, Phys. Rev. B 17,
26The deviations from the 2D scaling functions observed for the
thickest film are different from those observed for the thinner films. With increasing x2D F˜⫹ for the thickest film exhibits much slower decrease than F˜⫹2D. This stems from the dimen-sional crossover, although the 3D limit analysis is not fully valid yet共Ref. 20兲. We believe that for the thickest film the 2D scaling analysis is still valid in a narrow field range near Hc2. Hc2 obtained from the 2D scaling analysis is plotted in Fig. 3. 27N. Werthamer, E. Helfand, and P.C. Hohenberg, Phys. Rev. 147,
28A.T. Dorsey, Phys. Rev. B 46, 8376共1992兲; R.T. Troy and A.T.
Dorsey, ibid. 47, 2715共1993兲.
29W.F. Skocpol and M. Tinkham, Rep. Prog. Phys. 38, 1049 共1975兲.
30U. Mizutani, Prog. Mater. Sci. 28, 97共1983兲.
31B.L. Gallagher, D. Greig, M. A. Howson, and A.A.M. Croxon, J.
Phys. F: Met. Phys. 13, 119共1983兲.
32G.F. Weir, M.A. Howson, B.L. Gallagher, and G.J. Morgan,
Phi-los. Mag. B 47, 163 共1983兲; G.J. Morgan and G.F. Weir, ibid. 47, 177共1983兲.
33G.F. Weir and G.J. Morgan, J. Phys. F: Met. Phys. 11, 1833 共1981兲.
34W.L. Jonson, J. Appl. Phys. 50, 1557 共1979兲; B. Schro¨der, W.